#------------------------------------------------------------------------------
#$Date: 2017-04-04 15:51:18 +0300 (Tue, 04 Apr 2017) $
#$Revision: 194778 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/27/4002717.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4002717
loop_
_publ_author_name
'Mączka, Mirosław'
'Gągor, Anna'
'Ptak, Maciej'
'Paraguassu, Waldeci'
'da Silva, Tercio Almeida'
'Sieradzki, Adam'
'Pikul, Adam'
_publ_section_title
;
 Phase Transitions and Coexistence of Magnetic and Electric Orders in the
 Methylhydrazinium Metal Formate Frameworks
;
_journal_issue                   5
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2264
_journal_paper_doi               10.1021/acs.chemmater.6b05249
_journal_volume                  29
_journal_year                    2017
_chemical_formula_sum            'C4 H10 N2 O6 Zn'
_chemical_formula_weight         247.51
_space_group_crystal_system      trigonal
_space_group_IT_number           161
_space_group_name_Hall           'R 3 -2"c'
_space_group_name_H-M_alt        'R 3 c :H'
_symmetry_space_group_name_Hall  'R 3 -2"c'
_symmetry_space_group_name_H-M   'R 3 c :H'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   8.0633(3)
_cell_length_b                   8.0633(3)
_cell_length_c                   22.2638(10)
_cell_measurement_reflns_used    3715
_cell_measurement_temperature    180(1)
_cell_measurement_theta_max      29.2200
_cell_measurement_theta_min      3.4410
_cell_volume                     1253.59(9)
_computing_cell_refinement       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      179.91(18)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.6249
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.962
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Atlas'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0165
_diffrn_reflns_av_unetI/netI     0.0113
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.962
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            5061
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.962
_diffrn_reflns_theta_full        28.000
_diffrn_reflns_theta_max         29.470
_diffrn_reflns_theta_min         3.444
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    2.942
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.90336
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.41 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    1.967
_exptl_crystal_description       prism
_exptl_crystal_F_000             756
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.194
_refine_diff_density_min         -0.267
_refine_diff_density_rms         0.047
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.28(5)
_refine_ls_extinction_coef       0.0011(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.073
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     51
_refine_ls_number_reflns         698
_refine_ls_number_restraints     9
_refine_ls_restrained_S_all      1.076
_refine_ls_R_factor_all          0.0141
_refine_ls_R_factor_gt           0.0133
_refine_ls_shift/su_max          0.018
_refine_ls_shift/su_mean         0.004
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0160P)²+1.4300P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0335
_refine_ls_wR_factor_ref         0.0338
_reflns_Friedel_coverage         0.987
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.962
_reflns_number_gt                670
_reflns_number_total             698
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cm6b05249_si_002.cif
_cod_data_source_block           Zn180
_cod_depositor_comments
'Adding full bibliography for 4002715--4002727.cif.'
_cod_original_cell_volume        1253.59(11)
_cod_database_code               4002717
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_oxdiff_exptl_absorpt_empirical_full_min 0.921
_oxdiff_exptl_absorpt_empirical_full_max 1.111
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, z+1/2'
'-x+y, y, z+1/2'
'x, x-y, z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'-y+2/3, -x+1/3, z+5/6'
'-x+y+2/3, y+1/3, z+5/6'
'x+2/3, x-y+1/3, z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-y+1/3, -x+2/3, z+7/6'
'-x+y+1/3, y+2/3, z+7/6'
'x+1/3, x-y+2/3, z+7/6'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
N1 N 0.7475(19) 0.334(4) 0.0825(6) 0.0176(10) Uani 0.3333 1 d D U P
H1A H 0.8740 0.4102 0.0810 0.021 Uiso 0.3333 1 calc R U P
H1B H 0.7229 0.2138 0.0790 0.021 Uiso 0.3333 1 calc R U P
C2 C 0.6628(19) 0.3775(18) 0.0324(6) 0.024(3) Uiso 0.3333 1 d D . P
H2A H 0.5261 0.3104 0.0369 0.036 Uiso 0.3333 1 calc R U P
H2B H 0.6961 0.3384 -0.0042 0.036 Uiso 0.3333 1 calc R U P
H2C H 0.7098 0.5129 0.0312 0.036 Uiso 0.3333 1 calc R U P
N2 N 0.678(4) 0.357(3) 0.1414(4) 0.017(3) Uiso 0.3333 1 d D . P
H2D H 0.5585 0.2578 0.1470 0.025 Uiso 0.3333 1 d R U P
H2E H 0.6714 0.4657 0.1440 0.025 Uiso 0.3333 1 d R U P
Zn1 Zn 0.3333 0.6667 0.16887(16) 0.01071(13) Uani 1 3 d S T P
O1 O 0.5594(5) 0.6820(4) 0.22061(6) 0.0167(8) Uani 1 1 d . . .
O2 O 0.3500(4) 0.4609(5) 0.11513(7) 0.0166(7) Uani 1 1 d . . .
C1 C 0.5462(6) 0.5532(5) 0.2554(3) 0.0157(4) Uani 1 1 d . . .
H1 H 0.4250 0.4483 0.2619 0.019 Uiso 1 1 calc R U .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C2 N1 N2 113.8(13) . .
C2 N1 H1A 108.8 . .
N2 N1 H1A 108.8 . .
C2 N1 H1B 108.8 . .
N2 N1 H1B 108.8 . .
H1A N1 H1B 107.7 . .
N1 C2 H2A 109.5 . .
N1 C2 H2B 109.5 . .
H2A C2 H2B 109.5 . .
N1 C2 H2C 109.5 . .
H2A C2 H2C 109.5 . .
H2B C2 H2C 109.5 . .
N1 N2 H2D 108.6 . .
N1 N2 H2E 112.9 . .
H2D N2 H2E 106.7 . .
O2 Zn1 O2 90.85(17) . 3_565
O2 Zn1 O2 90.85(17) . 2_665
O2 Zn1 O2 90.85(17) 3_565 2_665
O2 Zn1 O1 178.5(2) . 2_665
O2 Zn1 O1 88.31(12) 3_565 2_665
O2 Zn1 O1 87.86(12) 2_665 2_665
O2 Zn1 O1 88.31(12) . 3_565
O2 Zn1 O1 87.86(12) 3_565 3_565
O2 Zn1 O1 178.5(2) 2_665 3_565
O1 Zn1 O1 92.96(16) 2_665 3_565
O2 Zn1 O1 87.86(12) . .
O2 Zn1 O1 178.5(2) 3_565 .
O2 Zn1 O1 88.31(12) 2_665 .
O1 Zn1 O1 92.96(16) 2_665 .
O1 Zn1 O1 92.96(16) 3_565 .
C1 O1 Zn1 125.1(2) . .
C1 O2 Zn1 125.2(2) 12_454 .
O2 C1 O1 124.77(19) 18_554 .
O2 C1 H1 117.6 18_554 .
O1 C1 H1 117.6 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
N1 C2 1.440(15) .
N1 N2 1.470(18) .
N1 H1A 0.8900 .
N1 H1B 0.8900 .
C2 H2A 0.9600 .
C2 H2B 0.9600 .
C2 H2C 0.9600 .
N2 H2D 0.9036 .
N2 H2E 0.9103 .
Zn1 O2 2.104(4) .
Zn1 O2 2.104(4) 3_565
Zn1 O2 2.104(4) 2_665
Zn1 O1 2.107(4) 2_665
Zn1 O1 2.107(4) 3_565
Zn1 O1 2.107(4) .
O1 C1 1.258(7) .
O2 C1 1.243(7) 12_454
C1 O2 1.243(7) 18_554
C1 H1 0.9300 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N1 H1A O2 0.89 2.07 2.85(2) 146.8 3_665
N1 H1B O1 0.89 2.00 2.83(2) 152.9 11_544
N1 H1B O2 0.89 2.41 3.19(2) 146.5 2_655
C2 H2A O1 0.96 2.17 3.115(14) 168.9 12_454
C1 H1 O1 0.93 2.58 3.160(7) 121.2 3_565
